 coefficient $C$ and explain how it increases substantially at small twist angles. To verify the validity of our theory, we also numerically evaluate the resistivity in the full temperature range (i.e. $T\gg{T_\text{BG}}$ as well as $T\ll{T_\text{BG}}$), and estimate the crossover temperature above which this enhanced linear-in-$T$ resistivity regime applies.

Resistivity from Boltzmann transport theory
-------------------------------------------

To begin with, we recall that in the Boltzmann transport theory the energy-averaged scattering time $\tau$ in monolayer graphene in the limit of $k_BT\ll \varepsilon_F$ is given by [@Min2011] $$\begin{aligned}
    {\langle\tau\rangle}^{-1} = \dfrac{2\pi}{\hbar}\nu_0\lvert W(k_F)\rvert^2 I, \label{Eq:ScatteringTime}\end{aligned}$$ where $\nu_0$ is the DOS per spin and valley at the Fermi energy, and $\lvert W(k_F)\rvert^2 = D^2\hbar k_F/(2\rho_m {v_\text{ph}})$ is the squared matrix element for acoustic phonon scattering. Here $\rho_m=\SI{7.6e-8}{g/cm^2}$ is the mass density of a single graphene sheet, ${v_\text{ph}}=\SI{2.6e6}{cm/s}$ is the phonon velocity in monolayer graphene, $D=\SI{25}{eV}$ is the acoustic phonon deformation potential [@Min2011], and $v_F$ is the Fermi velocity. The integral $I$ has the following form, $$\begin{aligned}
    I = \int \dfrac{\phi}{2\pi} \dfrac{F(q)(1-\cos\phi)}{\epsilon^2(q)} \dfrac{2q}{k_F}\beta \hbar\omega_q N_q(N_q+1), \label{Eq:IntegralI}\end{aligned}$$ where $q = 2k_F \sin(\phi/2)$ is the magnitude of the acoustic phonon wave vector, $\beta = 1/(k_B T)$, and $F(q)$ is the chiral factor defined as the square of the wave function overlap between incoming and scattered electrons. In addition, $N_q = (e^{\beta
coefficient $ C$ and explain how it increases substantially at small device angle. To verify the validity of our theory, we besides numerically evaluate the resistivity in the full temperature scope (i.e. $ T\gg{T_\text{BG}}$ as well as $ T\ll{T_\text{BG}}$), and estimate the crossing over temperature above which this enhanced linear - in-$T$ electric resistance regime applies. 

 Resistivity from Boltzmann transport theory 
 ------------------------------------------- 

 To get down with, we recall that in the Boltzmann transport hypothesis the energy - average dispersion time $ \tau$ in monolayer graphene in the limit of $ k_BT\ll \varepsilon_F$ is given by   [ @Min2011 ] $ $ \begin{aligned } 
     { \langle\tau\rangle}^{-1 } = \dfrac{2\pi}{\hbar}\nu_0\lvert W(k_F)\rvert^2 I, \label{Eq: ScatteringTime}\end{aligned}$$ where $ \nu_0 $ is the DOS per tailspin and valley at the Fermi energy, and $ \lvert W(k_F)\rvert^2 = D^2\hbar k_F/(2\rho_m { v_\text{ph}})$ is the squared matrix element for acoustic phonon dispersion. Here $ \rho_m=\SI{7.6e-8}{g / cm^2}$ is the mass concentration of a single graphene tabloid, $ { v_\text{ph}}=\SI{2.6e6}{cm / s}$ is the phonon velocity in monolayer graphene, $ D=\SI{25}{eV}$ is the acoustic phonon deformation potential   [ @Min2011 ], and $ v_F$ is the Fermi speed. The integral $ I$ has the following form, $ $ \begin{aligned } 
     I = \int \dfrac{\phi}{2\pi } \dfrac{F(q)(1-\cos\phi)}{\epsilon^2(q) } \dfrac{2q}{k_F}\beta \hbar\omega_q N_q(N_q+1), \label{Eq: IntegralI}\end{aligned}$$ where $ q = 2k_F \sin(\phi/2)$ is the magnitude of the acoustic phonon wave vector, $ \beta = 1/(k_B T)$, and $ F(q)$ is the chiral factor defined as the square of the wave function overlap between incoming and scattered electrons. In addition, $ N_q = (e^{\beta
 coffficient $C$ and explain mow it increases substaitially at smalu twist angles. To verify the vqlidiuj of our theory, we alro numeribally evaouatt the resistivity in the nbll tslperctnre range (i.e. $T\gn{T_\text{BG}}$ as well as $T\ll{T_\taxg{BY}}$), and estimate the crossover temperaeure abpvf which this eghanbeq lihvav-in-$T$ resistivity regime applies.

Rssistivpty from Boltzmanm transport theory
-------------------------------------------

To begin witj, we recall that ij the Boltznann rransport thdory the energy-averages scattering time $\tau$ in monolaher gxaphene in jkw llkit of $k_BT\lo \varvpsilon_F$ is glnen by [@Mhn2011] $$\begim{aligned}
    {\lakgle\teu\rabgle}^{-1} = \dfrac{2\pi}{\hbar}\nu_0\lvxrt W(k_F)\rvert^2 I, \label{Gq:ScatteritgCime}\end{aligned}$$ where $\bu_0$ is tve DMS pde soin aid balley at the Fermi energy, and $\lvert W(k_F)\rvert^2 = D^2\hnaw k_F/(2\rho_m {v_\text{lh}})$ is ehq squared matrix element for acoustic pvonkn scattering. Here $\rho_m=\WI{7.6e-8}{g/cm^2}$ is the mass dejsity of w single graphene sheet, ${v_\text{ph}}=\SI{2.6e6}{cm/s}$ is the phonmn vemuciuy in mubopayer graphene, $D=\SI{25}{eV}$ is the acoustic phonon dqrotmstion potentiaj [@Min2011], and $v_F$ id yre Fermi velozity. Tks jntegral $I$ has the followyng firm, $$\begin{wligmed}
    I = \int \dfrac{\phi}{2\pi} \dfeac{F(q)(1-\cos\phi)}{\eisilin^2(q)} \dfrac{2q}{k_F}\beta \hyar\omega_q N_q(U_q+1), \labgl{Eq:InyegralI}\end{aligned}$$ where $q = 2i_F \sin(\phi/2)$ id the maghktude of the acojstpc pvonon wave vector, $\beta = 1/(k_B T)$, and $F(q)$ is che chirxl fsctor qefined as the square of the wave vunctnon oeerlap betaeen incoming and scattered elervrons. In addijiot, $N_x = (e^{\beta
coefficient $C$ and explain how it increases small angles. To the validity of evaluate resistivity in the temperature range (i.e. as well as $T\ll{T_\text{BG}}$), and estimate crossover temperature above which this enhanced linear-in-$T$ resistivity regime applies. Resistivity from Boltzmann theory ------------------------------------------- To begin with, we recall that in the Boltzmann transport theory energy-averaged time in graphene in the limit of $k_BT\ll \varepsilon_F$ is given by [@Min2011] $$\begin{aligned} {\langle\tau\rangle}^{-1} = \dfrac{2\pi}{\hbar}\nu_0\lvert W(k_F)\rvert^2 \label{Eq:ScatteringTime}\end{aligned}$$ where $\nu_0$ is the DOS per spin valley at the Fermi and $\lvert W(k_F)\rvert^2 = D^2\hbar {v_\text{ph}})$ the squared element acoustic scattering. Here $\rho_m=\SI{7.6e-8}{g/cm^2}$ the mass density of a single graphene sheet, ${v_\text{ph}}=\SI{2.6e6}{cm/s}$ is the phonon velocity in monolayer graphene, $D=\SI{25}{eV}$ the acoustic potential [@Min2011], $v_F$ the velocity. The integral the following form, $$\begin{aligned} I = \dfrac{2q}{k_F}\beta \hbar\omega_q N_q(N_q+1), \label{Eq:IntegralI}\end{aligned}$$ where $q = 2k_F is the of the acoustic phonon wave vector, = 1/(k_B T)$, and $F(q)$ is the chiral defined as the square of the wave function overlap between incoming and scattered electrons. In = (e^{\beta
 coefficient $C$ and explain how It increaseS subsTanTiaLlY at sMall Twist angles. To vERify The validity of our theory, We alsO nUMeriCAlLy evaLuate thE ReSIStiViTy In tHe FUlL tempEraTure ranGe (i.e. $T\gg{T_\teXt{Bg}}$ aS well as $T\ll{T_\tEXt{bG}}$), and estimAte The crossover TemPeratuRe AboVE whicH thIs enhAnced lINear-in-$t$ resistivItY Regime APplies.

RESIsTiviTy from Boltzmann trANsPOrt theory
-------------------------------------------

To begIn with, We REcALL thAt iN the BoltzmAnN tranSPort theORy THE EneRGy-averaged scaTtering time $\TAu$ iN monolAyEr gRAphene In the LiMIt oF $k_BT\ll \varepSiloN_F$ is given By [@Min2011] $$\bEGin{aligNEd}
    {\langlE\tau\raNglE}^{-1} = \dfRac{2\pI}{\HbAr}\Nu_0\lVeRT W(k_f)\RvErt^2 i, \LabEl{Eq:ScatTeRiNgTimE}\end{ALIGNed}$$ wHerE $\nu_0$ iS the DoS per spin and vAllEy at THe FErmi eNergy, And $\lVeRt W(k_F)\Rvert^2 = D^2\Hbar k_f/(2\rHo_m {v_\text{ph}})$ is the SquaRed matrix EleMeNt fOr AcousTIc phonOn sCatTering. HEre $\rho_m=\si{7.6e-8}{g/Cm^2}$ IS THe Mass density of a singLe GRApHene sheeT, ${v_\text{PH}}=\Si{2.6e6}{CM/s}$ is the pHoNon VeloCITy in mOnolAYeR graphenE, $D=\SI{25}{eV}$ IS tHe AcoustiC pHonon dEfOrmAtiOn potENtiaL [@Min2011], anD $v_F$ is the fermi VElocity. The inteGRal $I$ has the folLOwING fORm, $$\beGin{Aligned}
    I = \int \DfraC{\Phi}{2\pI} \dfrAC{F(Q)(1-\coS\Phi)}{\epSilon^2(Q)} \dFRaC{2Q}{k_F}\beta \hbar\omega_q N_q(n_q+1), \Label{EQ:InteGralI}\end{alignEd}$$ where $q = 2k_F \SIN(\Phi/2)$ is the MagnITuDE of the acoustic PhonoN wave vectoR, $\Beta = 1/(k_B T)$, aNd $F(q)$ iS the chirAl factor dEFIned as thE sqUarE of The WAVe Function overlAP BetwEeN incomiNg aNd scattEreD elEctRonS. IN addition, $n_q = (e^{\beta
 coefficient $C$ and expla in how itincre ase s s ub stan tial ly at small tw i st a ngles. To verify the v alidi ty of o u rtheor y, we a l so n ume ri ca lly  e v al uatethe  resist ivity in t hefu ll temperatu r erange (i.e . $ T\gg{T_\text {BG }}$ as  w ell as $T \ll {T_\t ext{BG } }$), a nd estima te the cr o ssovert e mp erat ure above which t h is enhanced linea r-in-$ T$ re s i sti vit y regime a pp lies. 
Resist i vi t y fro m  Boltzmann tr ansport the o ry------ -- --- - ------ ----- -- - --- ----------- ---
To begin  with, we reca l l thatin the  Bo ltz mann tr an spo rt the o ry  th e  en ergy-ave ra ge d sca tter i n g time  $\ tau$  in m onolayer grap hen e in the  limi t of$k_B T\ ll \v arepsi lon_F $is given by [@M in20 11] $$\be gin {a lig ne d}
  {\lan gle \ta u\rangl e}^{-1} = \ df r a c {2 \pi}{\hbar}\nu_0\l ve r t  W (k_F)\rv ert^2I ,\l a bel{Eq:S ca tte ring T i me}\e nd{a l ig ned}$$ w here $ \ nu _0 $ is th eDOS pe rspi n a nd va l leyat the  Fermi e nergy ,  and $\lvert W ( k_F)\rvert^2=  D ^ 2 \h b ar k _F/ (2\rho_m {v _\te x t{ph }})$ is  th e  squa red m at r ix element for acousti cphonon  scat tering. Here$\rho_m=\S I { 7 .6e-8}{g /cm^ 2 }$ is the mass de nsity  of a sing l e graphe ne sh eet, ${v _\text{ph } } =\SI{2.6 e6} {cm /s} $ i s th e phonon velo c i ty i nmonolay ergraphen e,$D= \SI {25 }{ eV}$ is t he acous ti cph on ondefor m ation po te nti al  [@ Min20 1 1], an d $v_ F$ i sth e  Fe rmi vel o ci t y . Th ein tegr al$I $ has  the fol lowingform, $$\ beg i n{al ig ne d}
   I = \int \dfr ac {\phi}{2\p i}  \d frac{F ( q )(1-\cos \phi)}{\epsilon^2(q)} \ d frac{2q }{k _F}\b eta\hbar\ome ga_ q N_q( N_q + 1), \l abel{E q:Int eg ral I } \end{ a l ig ned }$ $ where $q =  2k _F \s in (\ph i/2)$ i s the magnitude of the  acoustic pho non  wav e ve cto r ,$ \be ta = 1 / ( k_B T)$, and $F (q)$ is th ec hi ral factor def in ed as t he squa re of the wav e functio n overlap  b etwe e n  in coming and  scatter ed electr o ns. I n  a dditi on,  $N_q=(e^ {\bet a
 coefficient_$C$ and_explain how it increases_substantially at_small_twist angles._To_verify the validity_of our theory,_we also numerically evaluate_the resistivity in_the_full temperature range (i.e. $T\gg{T_\text{BG}}$ as well as $T\ll{T_\text{BG}}$), and estimate the crossover temperature_above_which this_enhanced_linear-in-$T$_resistivity regime applies.

Resistivity from Boltzmann_transport theory
-------------------------------------------

To begin with, we_recall that_in the Boltzmann transport theory the energy-averaged scattering_time_$\tau$ in monolayer_graphene in the limit of $k_BT\ll \varepsilon_F$ is given_by [@Min2011] $$\begin{aligned}
    {\langle\tau\rangle}^{-1}_= \dfrac{2\pi}{\hbar}\nu_0\lvert W(k_F)\rvert^2_I,_\label{Eq:ScatteringTime}\end{aligned}$$_where $\nu_0$ is the_DOS per spin and valley at_the Fermi energy, and $\lvert W(k_F)\rvert^2_= D^2\hbar k_F/(2\rho_m {v_\text{ph}})$ is the squared_matrix element for acoustic phonon scattering._Here $\rho_m=\SI{7.6e-8}{g/cm^2}$ is the mass_density of_a single graphene sheet, ${v_\text{ph}}=\SI{2.6e6}{cm/s}$_is the phonon_velocity in_monolayer graphene, $D=\SI{25}{eV}$_is the acoustic phonon deformation potential [@Min2011],_and $v_F$ is_the Fermi velocity. The integral $I$_has_the following form,_$$\begin{aligned}
__ _I = \int_\dfrac{\phi}{2\pi}_\dfrac{F(q)(1-\cos\phi)}{\epsilon^2(q)} \dfrac{2q}{k_F}\beta_\hbar\omega_q_N_q(N_q+1), \label{Eq:IntegralI}\end{aligned}$$ where $q = 2k_F_\sin(\phi/2)$_is the magnitude of the acoustic phonon_wave vector, $\beta =_1/(k_B_T)$, and $F(q)$ is_the chiral factor defined as_the square of the wave function_overlap between_incoming and_scattered electrons. In addition, $N_q = (e^{\beta